Studies in Surface Science and Catalysis J.J. Spivey, E. Iglesia and T.H. Fleisch(Editors) 9 2001 Elsevier Science B.V. All rights reserved.
Catalytic Properties of Supported MoO3 Catalysts for Oxidative Dehydrogenation of Propane Kaidong Chen, Enrique Iglesia and Alexis T. Bell Chemical and Materials Sciences Divisions, Lawrence Berkeley National Laboratory, and Department of Chemical Engineering, University of California, Berkeley, CA 94720 The effects of MoOx structure on propane oxidative dehydrogenation (ODH) rates and selectivity were examined on A12Oa-supported MoOx catalysts with a wide range of surface density (0.4-12 Mo/nm2), and compared with those obtained on MoOx/ZrO2. On MoOx/A1203 catalysts, propane turnover rate increased with increasing Mo surface density and reached a maximum value for samples with -~ 4.5 Mo/nm 2. All MoOx species are exposed at domain surfaces for Mo surface densities below 4.5 Mo/nm 2. Therefore, the observed trends reflect an increase in ODH turnover rates with increasing MoOx surface density. As Mo surface densities increase above the polymolybdate monolayer value (-~ 4.5 Mo/nm2), ODH turnover rates decreased with increasing Mo surface density, as a result of the formation of MoO3 crystallites with inaccessible MoOx species. The ratio of rate constants (k2/kl) for propane combustion (k2) and for propane ODH reactions (kl) decreased with increasing MoOx surface density and then remained constant for values above 5 Mo/nm 2. Propene combustion rate constants (k3) also decreased relative to those for propane ODH (kl) as two-dimensional structures formed with increasing Mo surface density. These Mo surface density effects on k2/kl and ka/kl ratios were similar on MoO3/AI203 and MoOa/ZrO2, but the effects of Mo surface density on ODH turnover rates for samples with submonolayer MoOx contents were opposite on the two catalysts. A comparison of ODH reaction rates and selectivity among MoO3/A1203, MoO3/ZrO2, bulk MOO3, ZrM0208, and A12(MoO4)3 suggests that the behavior of supported MoOx at low surface densities resembles that for the corresponding bulk compounds (ZrM02Os, and A12(MoO4)3), while at high surface density the behavior approaches that of bulk MoO3 on both supports. 1. INTRODUCTION Many recent studies have explored the oxidative dehydrogenation of light alkanes as a potential route to the corresponding alkenes. Oxidative dehydrogenation (ODH) of alkanes is favored thermodynamically and the presence of 02 leads to the continuous removal of carbon deposits and to stable reaction rates. Secondary combustion reactions, however, limit alkene yields. For propane oxidative dehydrogenation reactions, the most active and selective catalysts are based on vanadium and molybdenum oxides [1-15]. On both V- and Mo-based catalysts, several studies of the kinetics and reaction mechanisms have shown that propane reactions occur via parallel and sequential oxidation steps (Scheme 1) [1-3, 11-14]. Propene forms via primary ODH reactions limited by the initial activation of the methylene C-H bond in propane (kl), while CO and CO2 (COx) can form via the combustion of the propene (k3) formed in step 1 or the primary combustion of propane (k2). The k2/kl ratio (propane
508 combustion/propane dehydrogenation) is usually low (-~0.1) for selective ODH catalysts . The alkene yield losses observed with increasing conversion arise, for the most part, from large k3/kl values (propene combustion/propane dehydrogenation- 10-50). These large k3/kl values reflect the weaker allylic C-H bond in propene relative to the methylene C-H bond in propane and the higher binding energy of alkenes on oxide surfaces [ 12-15]. The structure and propane ODH catalytic properties of ZrO2-supported MoO3 catalysts were recently described . A1203-supported MoO3 catalysts have been widely used in hydrodesulfurization, hydrogenation, and alkene metathesis reactions, and detailed studies of the structure of dispersed MoO3 on A1203 have been reported . In contrast, little is known about the reaction pathways and the structural requirements for propane ODH reactions on MoOx species supported on A1203 . This work addresses the effect of Mo surface density on the propane ODH properties for MoO3/A1203. The catalytic performance results obtained on MoO3/AI203 were compared with those reported previously on MoO3/ZrO2.
Scheme 1. Reaction network in oxidative dehydrogenation of propane 2. EXPERIMENTAL METHODS
A1203-supported MoOx samples were prepared by incipient wetness impregnation of 7-A1203 (Degussa, AG) with a solution of ammonium heptamolybdate (AHM) (99%, Aldrich, Inc.) at a pH of 5. Impregnated samples were dried overnight in air at 393 K and then treated in dry air (Airgas, zero grade) at 773 K for 3 h. ZrO2-supported MoOx samples were also prepared by incipient wetness impregnation method, as described elsewhere . Propane reaction rate and selectivity measurements were carried out at 703 K in a packed-bed tubular quartz reactor using 0.03-0.3 g samples. Propane (14 kPa; Airgas, 99.9%) and oxygen (1.7 kPa; Airgas, 99.999%) with He (Airgas, 99.999%) as a diluent were used as reactants. Reactants and products were analyzed by gas chromatography (Hewlett-Packard 5880 GC) using procedures described previously [13, 14]. C3Hs and 02 conversions were varied by changing reactant space velocity (F/w; w: catalyst mass; F: reactant volumetric flow rate). Typical conversions were < 2% for C3H8 and < 20% for 02. Initial ODH reaction rates and selectivities were obtained by extrapolation of these rate data to zero residence time. The effect of bed residence time on product yields was used in order to calculate rates and rate constants for secondary propene combustion reactions, using procedures reported previously [13,14]. 3. RESULTS AND DISCUSSION The structures of MoO3/A1203 and MoO3/ZrO2catalysts were characterized by BET surface area measurements, X-ray diffraction, and Raman, UV-visible, and X-ray absorption spectroscopy in previous studies [15, 16]. These data showed that the structure and domain size of MoOx species depend strongly on the Mo surface density and the temperature of treatment in air. For samples treated in dry air below 773 K and with Mo surface densities
509 below "monolayer" values (--4.5 Mo/nm2), only two-dimensional MoOx oligomers are detected on A1203 or ZrO2 surface. As Mo surface densities exceed this monolayer coverage, crystalline MoO3 forms. The size of the MoOx domains increased gradually with increasing Mo surface density. Propane ODH on Mo-based catalysts occurs via parallel and sequential oxidation pathways (Scheme 1) . The reaction rate constants (kl, k2 and k3) in Scheme 1 can be calculated from the effects of reactant residence time on propene selectivity . Propene yields during propane ODH reactions depend on both k2/kl and ka/kl; smaller values of either ratio lead to higher propene selectivity at a given propane conversion. Figure 1 shows the effects of Mo surface density o n k2/k I and k3/k 1 values for MoO3/A1203 catalysts. The value of kE/kl reflects the relative rates of initial propane combustion and dehydrogenation. The values of k2/kl decreased with increasing Mo surface density, until it reached a constant value of -0.05 for surface densities above 5 Mo/nm 2 (Figure l(a)). This gradual decrease in k2/kl values with increasing MoOx surface density suggests that Mo-O-A1 sites or uncovered A1203 surfaces near MoOx species catalyze the unselective conversion of propane to COx. This may reflect, in turn, the tendency of such sites to bind alkoxide intermediates more strongly than Mo-O-Mo structures in polymolybdate domains or on the surface of MoO3 clusters. The complete coverage of A1203 surfaces by a polymolybdate monolayer leads to a high initial propene selectivity, which resembles that in samples with predominantly MoO3 species. A similar decrease in k2/kl with increasing surface density of the active oxide was reported previously on MoOx/ZrO2  and VOx/AI203  catalysts. 1
_ _ _
Mo Surface Density (Molnm 2)
Mo Surface Density (Molnm 21
Fig. 1. Dependenceof (a) k2/kl, and (b) k3/k1on Mo surface density for MOOx/AI203 [ 14 kPa C3Hs, 1.7 kPa 02, balance He, 703 K] The values of k3/kl were much greater than unity on all MoOx/A1203 samples (Figure l(b)), indicating that propene combustion occurs much more rapidly than propane dehydrogenation. It is this large value that causes the significant decrease in propene selectivity with increasing propane conversion. The values of k3/kl (10-40) on these MoOx/A1203 catalysts are similar to those measured on MoOx/ZrO2 . The k3/kl ratio decreased with increasing Mo surface density and then remained constant for Mo surface densities above 5 Mo/nm 2. The large k3/kl ratio reflects the weaker C-H bonds in propene
510 compared to those in propane, as well as the higher binding energy of propene molecules on Lewis acid sites provided by Mo § cations present on MoO3 surfaces . Initial propane reaction rates are reported in Figure 2 as a function of Mo surface density on all MoOx/A1203 samples. Propane consumption rates normalized per Mo atom initially increased with increasing Mo surface density and they approached maximum values at surface densities of-- 4.5 Mo/nm 2 (Figure 2(a)). In this range of surface density, the accessibility of MoOx at domain surfaces is largely unaffected by Mo surface density, because the A1203 surface is covered predominantly by two-dimensional MoOx oligomers. Therefore, the observed increase in reaction rate reflects an increase in the reactivity (turnover rate) of exposed MoOx active sites with increasing domain size. Propane reaction rates decreased as Mo surface densities exceed-- 4.5 Mo/nm 2, which corresponds to the approximate surface density in a polymolybdate monolayer. The incipient appearance of three-dimensional MoO3 structures, with the consequent incorporation of MoOx into inaccessible positions within such clusters, is likely to account for the observed decrease in apparent turnover rates at higher surface densities (Figure 2(a)).
.. -t .....
-~- - -
el I e"
~ ,~ 0.4 (a)
Mo Surface Density (Mo/nm 2)
Mo Surface Density (Mo/nm 2)
Fig. 2. Effectsof Mo surface density on initial propane consumptionrate for MOOx/Al203 (a) normalized per Mo atoms, and (b) normalized per surface area. [ 14 kPa C3H8,1.7 kPa 02, balance He, 703 K] Figure 2(b)shows the propane consumption rates normalized per BET surface area. These areal rates initially increased sharply with increasing Mo surface density, but then remained almost constant for surface densities above 5 Mo/nm 2. Thus, it appears that the initial increase in propane turnover rates as two-dimensional structures grow reflects the increasing reactivity of MoOx surface structure on larger oxide domains. Similar domain size effects were observed on A1203-supported VOx catalysts . When Mo surface densities exceed monolayer coverages, three-dimensional MoO3 form and the entire surface of the catalyst becomes covered by either two-dimensional MoOx domains or MoO3 clusters with similar surface reactivity. Any additional MoOx species become inaccessible for propane ODH reactions; therefore, propane reaction rates normalized per Mo atom decreased, but areal rates remain constant with increasing MoOx surface density. The observed surface density effects on the catalytic, activity of MoOx/A1203 and MoOx/ZrO2 are different. On MoOx/ZrO2, propane turnover rates per Mo decreased with increasing Mo surface density, even below monolayer coverages . Figure 3(a) compares
511 propane consumption rates per Mo atom on MoOx/A1203 and MoOx/ZrO2. For Mo surface densities above ~ 5 Mo/nm 2, propane turnover rates on MoOx/A1203 and MoO~jZrO2 catalysts become similar, because in both cases catalyst surfaces are fully covered by two-dimensional or three-dimensional MoOx species. Below monolayer coverages (~5 Mo/nm2), however, propane turnover rates increased on MoOx/Al203 but they decreased on MoOx/ZrO2 with increasing surface density. Figure 3(b) shows the corresponding comparison for areal propane reaction rates on these two types of catalysts. Also shown in Figure 3(b) are areal rates on bulk ZrM0208, MoO3 and A12(MoO4)3. It appears from these data that the catalytic activity of the surface structures in bulk ZrMo2Os is considerable higher than on MoO3 surfaces, which in turn, is higher than that on A12(MoO4)3 surfaces. This suggests that active species with surface structures similar to those on the surface of ZrM0208 may also be more active than those resembling the surfaces of bulk MOO3, and more active still than those with surfaces resembling A12(MoO4)3. Since Mo surface densities in ZrM0208, MoO3 and A12(MoO4)3 are similar, propane turnover rates would follow a sequence similar to that of the areal rates shown in Figure 3(b) (ZrM0208 > MoO3 > AI2(MoO4)3). For low surface density samples, the structures of MoOx/Al203 and MoOx/ZrO2 surfaces would resemble those in the corresponding A12(MoO4)3 and ZrM0208 bulk phases. On MoOx/Al203 catalysts, the surface structure gradually changes from one resembling A12(MoO4)3 to one similar to MoO3 as the MoOx surface density increases. Therefore, propane turnover rates increase with increasing Mo surface density for values below monolayer coverages, as surface structures evolve from isolated species with significant Mo-O-A1 character to polymolybdate domains resembling in structure and in reactivity of the surface MoO3 (Figure 3(a)). In contrast, the surface structure of MoOx/ZrO2 evolves from one resembling ZrM0208 to one similar to MoO3 with increasing Mo surface density; as a result, propane turnover rates decrease with increasing Mo surface density (Figure 3(a)). 7
=i ~ e~ O ,,j
o Moo~A~0, MoO~Z~O,
~=. N E ~E e~ O W,
Mo Surface Density (Molnm z)
Fig. 3. Effects of Mo surface density on initial propane consumption rate on MoOx/Al203, MoOx/ZrO2, bulk ZrMo2Os, MoO3 and AI2(MoO4)3. (a) normalized per Mo atoms, and (b) normalized per surface area. [14 kPa C3H8, 1.7 kPa 02, balance He, 703 K]. Changes of k2/k] and k3/kl ratios as a function of Mo surface density on MoOx/A1203 and MoO• catalysts are consistent with the arguments presented above for the evolution of reaction rates with surface density on the two supports. Figure 4 shows k2/kl and k3/kl ratios on the supported MoOx catalysts and on bulk ZrM02Os, MoO3 and A12(MoO4)3. The
512 k2/kl and k3/kl ratios on A12(MoO4)3 and on ZrM0208 are higher than on MOO3. As Mo surface density increases, surface structures evolve from those resembling A12(MoO4)3 or ZrMo2Os surfaces to MoO3-1ike species; concurrently, k2/kl and k3/kl ratios decrease and approach those measured on MoO3 (Figures 4(a) and 4(b)). These results suggest that at low surface densities, supported MoOx species catalyze ODH reactions with turnover rates and selectivities strongly resembling those on the corresponding mixed oxide bulk structure. 1
~z, 9 4P
Mo Surface Density (Molnm 2)
Mo Surface Density (Molnm 2)
Fig. 4. Effectsof Mo surface density on (a) k2/k], and (b) k3/kI ratio for MOOx/AI203, MOOx/ZrO2, bulk ZrMo20s, MoO3 and AI2(MoO4)3. [ 14 kPa C3Hs, 1.7 kPa 02, balance He, 703 K]. ACKNOWLEDGEMENT
This work was supported by the Director, Office of Basic Energy Sciences, Chemical Sciences Division of the U.S. Department of Energy under Contract DE-AC03-76SF00098. REFERENCES
1. T. Blasko and J. M. L6pez Nieto, Appl. Catal. A 157 (1997) 117. 2. H. H Kung, Adv. Catal. 40 (1994) 1. 3. S. Albonetti, F. Cavani and F. Trifiro, Catal. Rev. -Sci. Eng. 38 (1996) 413. 4. G. Centi and F. Triffiro, Appl. Catal. A 143 (1996) 3. 5. E.A. Mamedov and V. Cort6s-Corberan, Appl. Catal. A 127 (1995) 1. 6. F.C. Meunier, A. Yasmeen and J. R. H. Ross, Catal. Today 37 (1997) 33. 7. L.E. Cadus, M. F. Gomez and M. C. AbeUo, Catal. Lett. 43 (1997) 229. 8. L. Jalowiecki-Duhamel, A. Ponchel and Y. Barbaux, J. Chim. Phys. PCB 94 (1997) 1975. 9. Y.S. Yoon, W. Ueda and Y. Moro-oka, Topics in Catal. 3 (1996) 256. 10. K. H. Lee, Y. S. Yoon, W. Ueda and Y. Moro-oka, Catal. Lett. 46 (1997) 267. 11. K. Chen, A. Khodakov, J. Yang, A. T. Bell and E. Iglesia, J. Catal. 186 (1999) 325. 12. K. Chen, A. T. Bell and E. Iglesia, J. Phys. Chem. B 104 (2000) 1292. 13. A. Khodakov, B. Olthof, A. T. Bell and E. Iglesia, J. Catal. 181 (1999) 205. 14. A. Khodakov, J. Yang, S. Su, E. Iglesia and A. T. Bell, J. Catal. 177 (1998) 343. 15. K. Chen, S. Xie, E. Iglesia and A. T. Bell, J. Catal. 189 (2000) 421. 16. K. Chen, S. Xie, A. T. Bell and E. Iglesia, J. Catal. in press.